**HAL Id: hal-01513860**

**https://hal.univ-lorraine.fr/hal-01513860**

Submitted on 30 Mar 2020
**HAL is a multi-disciplinary open access**

archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from

**L’archive ouverte pluridisciplinaire HAL, est**
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de

**An aﬀine formulation for the self-consistent modeling of**

**elasto-viscoplastic heterogeneous materials based on the**

**translated field method**

### Charles Moreau, Stéphane Berbenni

**To cite this version:**

Charles Moreau, Stéphane Berbenni. An aﬀine formulation for the self-consistent modeling of elasto-viscoplastic heterogeneous materials based on the translated field method. International Journal of Plasticity, Elsevier, 2015, 64, pp.134-150. �10.1016/j.ijplas.2014.08.011�. �hal-01513860�

## An affine formulation for the self-consistent

## modeling of elasto-viscoplastic heterogeneous

## materials based on the translated field

## method

### Charles Mareau

a### , St´ephane Berbenni

ba_{Arts et M´}_{etiers ParisTech, CER d’Angers, LAMPA, 2 bd du Ronceray, 49035}

Angers Cedex 1, France

b_{Laboratoire d’Etude des Microstructures et de M´}_{ecanique des Mat´}_{eriaux, LEM3,}

UMR CNRS 7239, University of Lorraine, Ile du Saulcy, 57045 Metz, France

Abstract

The modeling of heterogeneous materials with an elasto-viscoplastic behavior is generally complex because of the differential nature of the local constitutive law. Indeed, the resolution of the heterogeneous problem involves space-time couplings which are generally difficult to estimate. In the present paper, a new homogenization model based on an affine linearization of the viscoplastic flow rule is proposed. First, the heterogeneous problem is written in the form of an integral equation. The purely thermoelastic and purely viscoplastic heterogeneous problems are solved indepen-dently using the self-consistent approximation. Using translated field techniques, the solutions of the above problems are combined to obtain the final self-consistent formulation. Then, some applications concerning two-phase fibre-reinforced compos-ites and polycrystalline materials are presented. When compared to the reference solutions obtained from a FFT spectral method, a good description of the overall response of heterogeneous materials is obtained with the proposed model even when the viscoplastic flow rule is highly non-linear. Thanks to this approach, which is en-tirely formulated in the real-time space, the present model can be used for studying the response of heterogeneous materials submitted to complex thermo-mechanical loading paths with a good numerical efficiency.

Key words: A. Microstructures, B. Elastic-viscoplastic material, B.

Fibre-reinforced composite, B. Polycrystalline material, C. Homogenization

1 Introduction

The self-consistent scheme is a common homogenization method that was developed to connect local deformation mechanisms to the overall behavior of heterogeneous disordered materials (Hershey, 1954; Kr¨oner, 1958). In the past decades, many efforts have been made to obtain extensions of the self-consistent approximation to the non-linear case. For heterogeneous materi-als with a rate-independent elastoplastic behavior, Kr¨oner (1961) proposed a model where the plastic strain is considered as a stress-free strain (i.e. eigen-strain). However, internal stresses are largely overestimated with this method which, like Taylor’s model (Taylor, 1938), leads to uniform plastic strains. As an alternative, Hill (1965) developed an incremental version of the self-consistent approximation. The constitutive equations are written in the form of a pseudo-linear relation such that it is possible to use the self-consistent approximation at each stage of a loading path. Extending Hill’s idea to the case of viscoplasticity, Hutchinson (1976) applied the self-consistent method by introducing a viscoplastic modulus which results from the linearization of the constitutive relation. This approach has been later modified by Molinari et al. (1987) and Lebensohn and Tom´e (1993) who proposed an alternative defi-nition of the viscoplastic modulus based upon a tangent, rather than secant, formulation. Later, a first order affine linearization procedure for non linear elastic, viscoplastic and elastoplastic composites and polycrystals was devel-oped by Masson et al. (2000). In particular, these authors showed that such a first order affine approximation implemented within a self-consistent frame-work improves the estimate of the effective behavior of non-linear polycrystals in comparison with the incremental formulation of Hill (1965).

The case of elasto-viscoplasticity raises additional difficulties due to the dif-ferential nature of the constitutive equations involving different orders of time derivation. Different possibilities have been explored to overcome these dif-ficulties. In the case of linear viscoelasticity, Hashin (1969) and Laws and McLaughlin (1978) have used the correspondence principle to propose a hered-itary approach. Indeed, the use of Laplace-Carson transforms allows separating time and space variables such that it is possible to define a single viscoelastic modulus in the Laplace-Carson space. The self-consistent problem is solved in the Laplace-Carson space before proceeding to the inversion to the real time space. Extensions to the non-linear case have been proposed by Rougier et al. (1994) and Masson and Zaoui (1999). The constitutive law is first linearized at each step of the deformation path. In this way, the considered problem is converted into a viscoelastic problem, which can be classically solved using the self-consistent or the Mori-Tanaka approximation in the Laplace-Carson space. While the theoretical foundations of this approach are robust, the numerical implementation is rather complex mostly because the inversion of Laplace-Carson transforms requires intensive computations. Recently, the results of an

enhanced affine formulation for two-phase composites were compared to nu-merical results obtained by the finite element method in Pierard and Doghri (2006) and Pierard et al. (2007).

In contrast with hereditary formulations, internal variable approaches can be preferred for the simplicity of their numerical implementation. Indeed, the res-olution of the heterogeneous problem is achieved in the real time space with some internal variables whose introduction in the strain and stress concen-tration relations allows remembering the material’s history. The first develop-ments were carried out by Weng (1981a,b) who adapted Kr¨oner’s model to the case of elasto-viscoplasticity. However, similarly to the original proposition of Kr¨oner (1961), internal stresses are largely overestimated with this method (Zaoui and Raphanel, 1993). This approach was later extended to the case of finite strains by Nemat-Nasser and Obata (1986) and Harren (1991). Mercier and Molinari (2009) used the additive interaction law developed by Molinari (Molinari et al., 1997; Molinari, 2002) to derive a self-consistent model based upon a tangent linearization of the viscoplastic flow rule. The additive inter-action law has been later adapted to build a finite strain elasto-viscoplastic self-consistent model for polycrystals (Wang et al., 2010). Recently, an in-ternal variable approach obtained from a variational method was developed by Lahellec and Suquet (2007a,b) to describe the behavior of composite ma-terials. Paquin et al. (1999), Sabar et al. (2002) and Berbenni et al. (2004) proposed an alternative framework based upon the specific properties of pro-jection operators. In the approach of Paquin et al. (1999), the purely elastic and purely viscoplastic heterogeneous problems are solved independently us-ing the self-consistent approximation. Usus-ing translated field techniques, the individual solutions are combined to deduce a strain rate localization rule. Comparisons between both the translated field techniques and the additive interaction law were reported in Mercier et al. (2012) in the case of two-phase compressible or incompressible linear viscoelastic composites using a Mori-Tanaka approximation.

In the present paper, an extension of the translated field approach initiated by Paquin et al. (1999) for the modeling of disordered materials using the self-consistent approximation is proposed. The motivations are twofold. First, while the original approach of Paquin et al. (1999) derives from a classical secant approximation, this work aims at adopting an affine linearization pro-cedure of the viscoplastic flow rule (i.e. a first order Taylor expansion of the viscoplastic flow rule) as suggested by Masson et al. (2000). Indeed, it has been observed that the first order affine formulation yields softer responses than the secant formulation (Masson and Zaoui, 1999; Masson et al., 2000; Molinari, 2002) which, in the case of pure viscoplasticity (or non linear elas-ticity in a general sense), may lead to the violation of a non-linear upper bound for the moduli (Gilormini, 1995). Second, in the original approach of Paquin et al. (1999), the local constitutive law only accounts for elastic and

viscoplastic contributions. In the present work, the contribution of thermal expansion is also considered so that the proposed model may be used to in-vestigate the response of disordered materials subjected to thermo-mechanical loading paths. Using the Mori-Tanaka approximation, a first order affine ex-tension to the model of Paquin et al. (1999) has already been proposed for two-phase materials by Berbenni and Capolungo (2014). It was shown that predictions are very close to the ones obtained with the incremental varia-tional approach developed by Lahellec and Suquet (2007b) for two-phase fibre-reinforced composites. It is also thought that such translated field approaches are simpler to formulate than the recent incremental variational approaches for non-linear elastic-viscoplastic materials (Brassard et al., 2012; Lahellec and Suquet, 2007b, 2013) whose development within a self-consistent framework for polycrystalline materials has not been achieved yet.

The paper is structured as follows. In the first section, starting from field equations, the heterogeneous problem is written in the form of an integral equation. Then, the translated fields, which are obtained from the solutions of the purely thermoelastic and purely viscoplastic heterogeneous problems, are introduced in order to simplify the integral equation. Finally, the localization rule associated with the proposed affine formulation is deduced from the appli-cation of the self-consistent method. As an illustration, some appliappli-cations are presented in the second section. The case of two-phase fibre-reinforced com-posites is first examined in order to compare the results from the proposed self-consistent approach with those given by others (Berbenni and Capolungo, 2014; Lahellec and Suquet, 2007b; Paquin et al., 1999). Then, the model is used to describe the behavior of polycrystalline materials when they are sub-jected to various thermomechanical loading conditions. To demonstrate the relevance of the proposed affine formulation, it is compared to the original classical secant formulation of Paquin et al. (1999) and to the full-field FFT spectral method of Moulinec and Suquet (1998).

2 Model description

2.1 Field equations

Considering a heterogeneous material, the proposed homogenization model aims at determining the macroscopic response of a representative volume ele-ment V which is submitted to some specific boundary conditions. The macro-scopic response is given by the relation between the macromacro-scopic stress rate and strain rate tensors ( ˙Σ and ˙E). The macroscopic stress rate and strain rate tensors are connected to the local stress rate and strain rate tensors ( ˙σ and ˙ε)

according to the classical averaging relations of homogenization theory: ˙Σ (t) = 1 V Z V ˙σ (x, t) dx =< ˙σ (t) > (1) ˙ E (t) = 1 V Z V ˙ε (x, t) dx =< ˙ε (t) > (2)

The determination of the local stress rate and strain rate fields is based on the resolution of the field equations associated with the heterogeneous problem. First, within the infinitesimal strain framework, the kinematical compatibility relation is given by:

˙ε (x, t) = ∇s˙u (x, t) (3)

where ˙u is the velocity field. In the absence of volume forces, static equilibrium conditions impose:

divσ (x, t) = 0 (4) div ˙σ (x, t) = 0 (5) Boundary conditions are prescribed on ∂V according to:

˙u (x, t) = ˙E (t) .x on ∂V (6) The decomposition of the total strain rate into themoelastic ( ˙εte) and

vis-coplastic ( ˙εvp) contributions leads to:

˙ε (x, t) = ˙εte(x, t) + ˙εvp(x, t) (7)

The thermoelastic strain rate results from a stress dependent contribution due to elasticity and a stress-independent contribution associated with thermal expansion ˙εth such that:

˙εte(x, t) = s (x, t) : ˙σ (x, t) + ˙εth(x, t) (8)

where s (with c = s−1_{) is the local elastic compliance tensor.}

In the general case, the viscoplastic strain rate is a non-linear function g depending on both the stress tensor σ and some internal variables denoted by β. For further use of the self-consistent approximation, the viscoplastic flow rule has to be linearized. Different linearization methods have been proposed. In the original approach of Paquin et al. (1999), the flow rule linearization is based upon a secant formulation. However, since the secant formulation is known to overestimate the stiffness (Gilormini, 1995; Masson and Zaoui, 1999; Masson et al., 2000), the affine linearization method is chosen here. In its linearized form, the viscoplastic strain rate is written:

˙εvp(x, t) = g (σ, β) ≈ mt(x, t) : σ (x, t) + ˙η (x, t) (9)

where mt (with bt= m−1t ) is the viscoplastic compliance tensor defined by:

m_{t}_{(x, t) =} ∂g (σ, β)

and ˙η corresponds to a back-extrapolated strain rate:

˙η (x, t) = g (σ, β) − mt(x, t) : σ (x, t) (11)

Thus, the final form of the constitutive law is:

˙ε (x, t) = s (x, t) : ˙σ (x, t) + ˙εth(x, t) + mt(x, t) : σ (x, t) + ˙η (x, t) (12)

The secant formulation proposed by Paquin et al. (1999) is retrieved when the tangent compliance tensor is replaced by the secant compliance tensor and by setting ˙η to zero. Because of the differential nature of the above constitu-tive law, the modeling of elasto-viscoplastic heterogeneous solids requires to deal with a space-time relation which does not exist for elastic, elastoplastic or viscoplastic heterogeneous solids. The next section aims at proposing an integral equation, which includes the space-time coupling associated with the elasto-viscoplastic constitutive model, to describe the heterogeneous problem.

2.2 Integral equation

To recast the heterogeneous problem in the form of an integral equation, the local elastic modulus c (respectively viscoplastic modulus bt) is expressed as

the sum of an uniform reference modulus C (respectively Bt) and a fluctuating

part δc (respectively δbt, the dependence with t is omitted):

c_{(x) = C + δc (x)} _{(13)}
b_{t}_{(x) = B}_{t}_{+ δb}_{t}_{(x)} _{(14)}
To obtain the integral equation, the modified Green operators ΓC and ΓBt

associated with the thermoelastic and viscoplastic reference media are now introduced. The modified Green operators ΓC and ΓBt

are defined as follows:

ΓC_{ijkl}(x − x′_{) = −}1
2
GC_{ik,jl}(x − x′_{) + G}C
jk,il(x − x′)
(15)
ΓBt
ijkl(x − x′) = −
1
2
GBt
ik,jl(x − x′) + GB
t
jk,il(x − x′)
(16)
where GC _{(respectively G}Bt) is the elastic (respectively viscoplastic) Green

function and, x and x′ _{are position vectors. The definition of Green functions}

can be found in many textbooks (Mura, 1987; Nemat-Nasser and Hori, 1994). As established by Kr¨oner (1989), the modified Green operators display the following properties for any compatible strain (or strain rate) field and any balanced stress (or stress rate) field (in the following, the dependence with x will be omitted):

ΓC ∗ ˙σ = 0 (17) ΓBt

ΓC : C∗ ˙ε = ˙ε − ˙E (19) ΓBt : Bt ∗ ˙ε = ˙ε − ˙E (20) where ∗ denotes the spatial convolution product. Using the specific properties of the modified Green operators (equations (17) to (20)) in combination with the constitutive model (equation (12)), the integral equation associated with the heterogeneous problem is obtained:

˙ε = ˙E−ΓC∗(δc : ˙εte− c : ˙εth)−ΓBt∗(δbt: ˙εvp− bt : ˙η)+ ΓC : C − ΓBt : Bt ∗ ˙εvp (21) The above integral equation, which contains the entire heterogeneous problem, is very similar to the one obtained by Paquin et al. (1999). The only difference lies in the choice of the linearization procedure. The integral equation shows how the local strain rate depends on both the macroscopic strain rate and the interactions between the different points of the representative volume element. In most cases, analytical solutions of this equation do not exist and some numerical procedures have to be used (e.g. spectral methods (Lebensohn et al., 2012; Moulinec and Suquet, 1998)). The self-consistent approximation, coupled with the translated field techniques, aims at estimating the unknown fields σ, ˙σ and ˙ε by considering only local interactions to simplify the integral equation. Following the approach of Paquin et al. (1999), the solutions of the purely elastic and purely viscoplastic heterogeneous problems will be used to introduce the translated fields in the integral equation.

2.3 Cases of pure thermoelasticity and pure viscoplasticity

Considering the same representative volume element with a purely thermoe-lastic behavior (i.e. ˙ε = s : ˙σ + ˙εth) or a purely viscoplastic behavior (i.e.

˙ε = mt : σ + ˙η), the integral equation (21) simplifies to:

˙ε = ˙E − ΓC∗ (δc : ˙ε − c : ˙εth) for pure thermoelasticity (22)

˙ε = ˙E − ΓBt

∗ (δbt : ˙ε − bt: ˙η) for pure viscoplasticity (23)

Introducing the strain rate concentration tensors associated with the elastic and viscoplastic reference media (AC and ABt

), the above equations become: ˙ε = AC : ˙E + AC : ΓC ∗ (c : ˙εth) for pure thermoelasticity (24)

˙ε = ABt

: ˙E + ABt

: ΓBt

∗ (bt: ˙η) for pure viscoplasticity (25)

where AC and ABt

are defined as the solutions of the following equations:

AC _{+ Γ}C_{∗}_{δc : A}C_{= I} _{(26)}
ABt
+ ΓBt
∗δbt: ABt
= I (27)

The macroscopic constitutive laws display the same structure as the local constitutive laws of the heterogeneous media such that:

˙Σ = Ce_{:}

˙ E − ˙Ethe

for pure thermoelasticity (28)

Σ = Be_{t} :E − ˙˙ Ne for pure viscoplasticity (29)
where Ce, Be_{t}, ˙Ee

th and ˙Ne are respectively the effective elastic modulus, the

effective viscoplastic modulus, the effective thermal strain rate and the ef-fective back-extrapolated strain rate of the heterogeneous solid with either a purely thermoelastic behavior or a purely viscoplastic behavior. The stress (rate) concentration rules are deduced from relations (24) and (25):

˙σ = c : AC : Se : ˙Σ + c : AC : ˙Ee th

+ c : AC : ΓC ∗ (c : ˙εth) − c : ˙εth for pure thermoelasticity

(30)

σ = bt: ABt : Met : Σ + bt: ABt : ˙Ne

+ bt: ABt : ΓBt ∗ (bt: ˙η) − bt: ˙η for pure viscoplasticity

(31)

with Se = Ce−1 and Me_{t} = Be−1_{t} . The averaging conditions < ˙ε >= ˙E,
< ˙σ >= ˙Σ and < σ >= Σ impose:
Ce _{=< c : A}C _{>} _{(32)}
Be
t =< bt: ABt > (33)
< AC >= I (34)
< ABt
>= I (35)
< AC : ΓC∗ (c : ˙εth) >= 0 (36)
< ABt
: ΓBt
∗ (bt: ˙η) >= 0 (37)
< c : ˙εth> −Ce : ˙Ethe =< c : AC : ΓC∗ (c : ˙εth) > (38)
< bt: ˙η > −Bet : ˙Ne=< bt: ABt : ΓBt∗ (bt: ˙η) > (39)

2.4 Introduction of the translated fields

The integral equation (21) can be simplified by using the solutions of the purely
thermoelastic and purely viscoplastic heterogeneous problems. Considering the
thermoelastic part of the strain rate, it can be decomposed into the solution
of the purely thermoelastic problem (denoted by ˙e′_{) and a residual strain rate}

field corresponding to the internal stress rate field ˙σ′_{:}

where ˙e′ _{is taken as the solution of the purely thermoelastic heterogeneous}

problem:

˙e′ _{=< ˙ε}

te > −ΓC∗ (δc : ˙e′− c : ˙εth) (41)

Adopting the same reasoning for the viscoplastic strain rate yields:

˙εvp = mt: σ + ˙η = ˙e′′+ mt : σ′′ (42)

where ˙e′′ _{is chosen as the solution of the purely viscoplastic heterogeneous}

problem:

˙e′′ _{=< ˙ε}

vp> −ΓBt∗ (δbt: ˙e′′− bt: ˙η) (43)

Because of the additive decomposition of the strain rate into thermoelastic and viscoplastic parts, one obtains:

˙ε = ˙εte+ ˙εvp = ˙e′+ ˙e′′+ ˙ε⋆ (44)

where ˙ε⋆ _{is the translated strain rate field associated to the translated stress}

(rate) fields ˙σ′ _{and σ}′′_{:}

˙ε⋆ = s : ˙σ′ _{+ m}

t: σ′′ (45)

The most interesting feature of this decomposition lies in the specific
proper-ties of the recently introduced translated fields. Indeed, ˙σ′ _{and σ}′′_{are balanced}

stress (rate) fields while ˙ε⋆ _{is compatible. Also, the importance of the }

trans-lated strain rate field ˙ε⋆ _{should be highlighted. According to equation (44),}

the total strain rate is decomposed into the thermoelastic solution ( ˙e′_{), the}

viscoplastic solution ( ˙e′′_{) and an additional contribution ( ˙ε}⋆_{) which represents}

the complexity of the space-time interactions associated with the
thermoelas-tic and viscoplasthermoelas-tic couplings. This treatment of the entire problem allows for
combining the separate solutions of the thermoelastic and viscoplastic
hetero-geneous problem without compromising the issue of their mutual interactions
which are described through ˙ε⋆_{.}

Based on the translated field properties, an associated problem, which is de-scribed by the following integral equation, is now considered:

˙ε⋆ _{= ˙}_{E}⋆_{−Γ}C_{∗(δc : s : ˙σ}′_{)−Γ}Bt
∗(δbt: mt: σ′′)+
ΓC : C − ΓBt
: Bt
∗(mt : σ′′)
(46)
where ˙E⋆ _{is the macroscopic strain rate field from which boundary conditions}

are prescribed on ∂V . Also, because of the properties given by equations (32) to (39), the following averaging relations are verified:

< ˙ε⋆ >= ˙E⋆ = 0 (47)
< s : ˙σ′ _{>= 0} _{(48)}
< mt: σ′′ >= 0 (49)
Se_{:< ˙σ}′ _{>=}_{S}e _{: ˙Σ + ˙}_{E}e
th
− < ˙εte >=< ˙εvp > − ˙Evpe (50)
Me
t :< σ′′ >=
Me
t : Σ + ˙Ne
− < ˙εvp > (51)

2.5 Self-consistent approximation

In order to solve the associated problem, which consists of equations (41), (43) and (46), the self-consistent approximation is used. The main idea of the self-consistent approximation is the decomposition of the modified Green op-erator ΓC (respectively ΓBt

) associated with the thermoelastic (respectively
viscoplastic) reference homogeneous medium into a local part (subscript l)
and a non-local part (subscript nl) to weaken the influence of non-local
inter-actions:
ΓC(x − x′_{) = Γ}C
l δ (x − x′) + ΓCnl(x − x′) (52)
ΓBt
(x − x′_{) = Γ}Bt
l δ (x − x′) + ΓB
t
nl (x − x′) (53)

The influence of non-local terms, which are difficult to estimate, is weakened by introducing uniform second-order tensors in the integral equations (41), (43) and (46). Indeed, for any uniform tensor X, the fields ABt

: X, AC : X and X are kinematically admissible while the fields c : AC : X and bt : ABt : X are

balanced. Thus, these different fields benefit from the specific properties of the modified Green operators ΓC and ΓBt

(relations (17) to (20)). Therefore, using the above decomposition of the modified Green operators and introducing the unknown uniform tensors (Y1 to Y5) in the integral equations (41), (43) and

(46) leads to:
˙ε⋆ = ˙E⋆− ΓC_{l} :δc : s : ˙σ′ _{− c : A}C _{: Y}
1
− ΓC_{nl}∗δc : s : ˙σ′ _{− c : A}C _{: Y}
1
− ΓBt
l :
δbt: mt : σ′′− bt: ABt : Y2
− ΓBt
nl ∗
δbt: mt : σ′′− bt: ABt : Y2
+ΓC_{l} : C − ΓBt
l : Bt
:m_{t}_{: σ}′′_{− A}Bt
: Y3
+ΓC_{nl} : C − ΓBt
nl : Bt
∗m_{t}_{: σ}′′_{− A}Bt
: Y3
(54)
˙e′ _{=< ˙ε}
te > −ΓCl : (δc : ˙e′− c : ˙εth+ C : Y4)
− ΓC_{nl}∗ (δc : ˙e′_{− c : ˙ε}
th+ C : Y4)
(55)
˙e′′_{=< ˙ε}
vp> −ΓBl t : (δbt: ˙e′′− bt : ˙η + Bt: Y5)
− ΓBt
nl ∗ (δbt : ˙e′′− bt : ˙η + Bt: Y5)
(56)
Neglecting the non-local terms requires to choose Y1, Y2, Y3, Y4 and Y5 such

that the following self-consistency conditions are fulfilled:

< δc : s : ˙σ′ _{− c : A}C _{: Y}
1 >= 0 so Y1 = Se:< ˙σ′ > (57)
< δbt: mt : σ′′− bt: ABt : Y2 >= 0 so Y2 = Met :< σ′′ > (58)
< mt: σ′′− ABt : Y3 >= 0 so Y3 = 0 (59)
< δc : ˙e′_{− c : ˙ε}
th+ C : Y4 >= 0 so C : Y4 = Ce: ˙Ethe (60)

< δbt : ˙e′′− bt : ˙η + Bt: Y5 >= 0 so Bt : Y5 = Bet : ˙Ne (61)

Considering only local terms and using the expressions of the unknown tensors, the self-consistent solution of the associated problem is given by:

˙ε⋆ = ˙E⋆− ΓCl :
δc : s : ˙σ′_{− c : A}C _{: S}e _{:< ˙σ}′ _{>}
− ΓBt
l :
δbt: mt: σ′′− bt : ABt : Met :< σ′′>
+ΓC_{l} : C − ΓBt
l : Bt
: (mt : σ′′)
(62)
˙e′ _{=< ˙ε}
te > −ΓCl :
δc : ˙e′_{− c : ˙ε}
th+ Ce : ˙Ethe
(63)
˙e′′ _{=< ˙ε}
vp > −ΓBlt :
δbt: ˙e′′− bt: ˙η + Bet : ˙Ne
(64)
Regarding the properties of the elastic and viscoplastic reference media, it
is imposed to choose the solutions obtained for the purely thermoelastic and
purely viscoplastic heterogeneous problems using the self-consistent
approxi-mation (i.e. C = Ce and Bt = Bet). This choice for the properties of the

ref-erence media is needed to ensure that the averaging relations < ˙e′ _{>=< ˙ε}
te >

and < ˙e′′ _{>=< ˙}_{ε}

vp> are verified.

Returning to the original problem, the strain rate concentration rule is ob-tained from the combination of equations (44), (62), (63) and (64):

˙ε = AC : ˙E + AC : ΓC_{l} :c _{: ˙ε}_{th}_{− C}e _{: ˙}_{E}e
th
+ AC : ΓBt
l :
b_{t} _{: ˙η − B}e
t : ˙Ne
+ AC : ΓC_{l} :δc : ˙εvp+ c : AC :< ˙εvp> − ˙Evpe
− AC : ΓBt
l :
δbt : ˙εvp− bt: ABt :
Me
t : Σ + ˙Ne− < ˙εvp>
+ AC :ΓC_{l} : Ce− ΓBt
l : Bet
:˙εvp− ABt :< ˙εvp>
− AC :ΓC_{l} : Ce− ΓBt
l : Bet
:ABt
: ΓBt
l :
b_{t}_{: ˙η − B}e
t : ˙Ne
(65)

The above relation describes the connection between ˙ε and ˙E as a function of the spatial interactions resulting from the thermal and viscoplastic incompat-ibilities. It is emphasized that only the self-consistent solutions of the purely thermoelastic and viscoplastic heterogeneous problems are needed to estimate the local strain rate and stress rate fields. Moreover, in contrast with the propositions of Rougier et al. (1994) and Masson and Zaoui (1999), no com-plex numerical procedure is involved since relations (63) to (65) are entirely formulated in the real-time space. Substituting the concentration rule (65) in the local constitutive equation (12) gives the following interaction law for

stresses:
˙σ = c : AC :Se _{: ˙Σ + ˙}_{E}e
vp+ ˙Ethe
− c : ˙εvp− c : ˙εth
+ c : AC : ΓCl :
c_{: ˙ε}_{th}_{− C}e _{: ˙}_{E}e
th
+ c : AC : ΓBt
l :
b_{t} _{: ˙η − B}e
t : ˙Ne
+ c : AC : ΓC_{l} :δc : ˙εvp+ c : AC :< ˙εvp > − ˙Evpe
− c : AC : ΓBt
l :
δbt: ˙εvp− bt: ABt :
Me
t : Σ + ˙Ne− < ˙εvp >
+ c : AC :ΓC_{l} : Ce− ΓBt
l : Bet
:˙εvp− ABt :< ˙εvp >
− c : AC :ΓC_{l} : Ce− ΓBt
l : Bet
:ABt
: ΓBt
l :
b_{t}_{: ˙η − B}e
t : ˙Ne
(66)
where ˙Ee

vp is the effective viscoplastic strain rate which is chosen to impose

the condition < ˙σ >= ˙Σ:
˙
E_{vp}e = Z :< c : ˙εvp > −Z :< c : AC : ΓBt
l :
b_{t}_{: ˙η − B}e
t : ˙Ne
>
− Z :< c : AC : ΓC_{l} :δc : ˙εvp+ c : AC :< ˙εvp >
>
+ Z :< c : AC : ΓBt
l :
δbt: ˙εvp− bt : ABt :
Me
t : Σ + ˙Ne− < ˙εvp >
>
− Z :< c : AC :ΓC_{l} : Ce− ΓBt
l : Bet
:˙εvp− ABt :< ˙εvp >
>
+ Z :< c : AC :ΓC_{l} : Ce− ΓBt
l : Bet
:ABt
: ΓBt
l :
b_{t} _{: ˙η − B}e
t : ˙Ne
>
(67)
with:
Z =I − Se :< c : AC : Γ_{l}C : c : AC >−1 : Se (68)

2.6 Particular case of two-phase materials

In the case of two-phase materials (with phases r = 1, 2), the Levin’s formula
(Levin, 1967) can be used to further simplify the strain rate concentration
equation (65) (see also Masson et al. (2000); Rekik et al. (2007)). Thus, for
each phase r = 1, 2, the expression of ˙e′(r) _{simplifies to:}

˙e′(r)= AC (r):< ˙εte > +aC (r) (69)

where aC (r) _{is given by:}

aC (r)=
AC (r)_{− I}
:c(2)_{− c}(1)−1 _{:}_{τ}_{te}(2)_{− τ}_{te}(1) _{(70)}
with τte(r) = −bt(r): ˙ε
(r)

th. In a similar manner, the expression of ˙e

′′_{(r)}
becomes:
˙e′′(r) = ABt(r)
:< ˙εvp> +aBt
(r)
(71)

where aBt(r) is given by:
aBt(r)
=
ABt(r)
− I
:b_{t}(2) _{− b}_{t}(1)−1 _{:}_{τ}_{vp}(2)_{− τ}_{vp}(1) _{(72)}

with τvp(r) = −bt(r) : ˙η(r). Thus, for two-phase materials, equation (65) can

be recast for each phase r = 1, 2 as (the superscript (r) is now removed to simplify the notations):

˙ε = AC : ˙E + aC + AC :ABt−1
: aBt
+ AC : ΓC_{l} :δc : ˙εvp+ c : AC :< ˙εvp > − ˙Evpe
− AC : ΓBt
l :
δbt: ˙εvp+ bt: ABt :<
δmt :
σ − τvp− bt: aBt
>
+ AC :ΓC_{l} : Ce− ΓBt
l : Bet
:˙εvp− ABt :< ˙εvp > −aBt
(73)
where ˙Ee

vp is obtained from equation (67) together with equation (73) and

averaging relations (1) and (2).

3 Applications

3.1 Fibre-reinforced composites

In order to study the effect of non-linear viscosity on the overall response, the present self-consistent (SC) approximation, which uses the translated field (TF) techniques together with a first order affine (AFF) linearization pro-cedure of the viscoplastic flow rule (equation (73), labeled as SC-TF-AFF), is applied to two-phase fibre-reinforced composites. The interest for study-ing such composite materials is twofold. First, a Mori-Tanaka approximation based on translated field techniques and coupled with a first order affine for-mulation (labeled as MT-TF-AFF) has been recently developed by Berbenni and Capolungo (2014). It is therefore interesting to compare the self-consistent and Mori-Tanaka schemes for two-phase composite materials with an elasto-viscoplastic behavior. Second, to observe the influence of the linearization procedure, the present SC-TF-AFF approach is also compared to the original self-consistent approach of Paquin et al. (1999) (labeled as SC-TF-SEC) which uses a secant approximation of the viscoplastic flow rule (Paquin et al., 1999).

The composite material is made of a matrix phase (r = M) and long cylin-drical fibres (r = I). Fibres are aligned along the same direction (x3) and are

perpendicular to the (x1, x2) plane. These microstructures were extensively

as SEC (EIV+HS)) developed for non-linear composites. This variational ap-proach consists of an incremental effective potential apap-proach where the in-ternal variables are the effective viscoplastic strain rates (i.e. EIV stands for ”Effective Internal Variable”) which are determined from a modified secant ap-proach. The effective properties of the thermoelastic-like homogeneous equiv-alent medium are obtained from the Hashin-Shtrikman (HS) estimates calcu-lated for the composite cylinder assemblage (CCA). For such fibre-reinforced composites, full-field FFT calculations have been performed earlier by Lahel-lec and Suquet (2007b) to obtain ”exact” solutions. Their results are used here as reference solutions to demonstrate the relevance of the present affine approach. The RVE studied by Lahellec and Suquet (2007b) for the FFT cal-culations is a 2D volume element where fibres are seen as a composite cylinder assemblage of self-similar cylinders.

Here, both phases are given an elasto-viscoplastic behavior (with ˙εth = 0).

The non-linear viscoplastic flow rule takes the form of a power law (Norton’s
model):
˙ε = s : ˙σ + 3
2ε˙0
σeq
σ(r)_{0}
!1/m
s
σeq
(74)
where m is the strain-rate sensitivity parameter which is the same for both
phases, s is the deviatoric stress, σeq is the Von Mises equivalent stress, ˙ε0 is

a reference strain rate and σ_{0}(r) is the flow stress for each phase (r).

The material parameters used for the simulations are the same as in Lahellec and Suquet (2007b) and Berbenni and Capolungo (2014) with a fibre volume fraction of f = 0.21. σ(M )0 = 1 GPa for the matrix while σ

(I) 0 = 5σ

(M )

0 for the

inclusions which are considered as hard fibres. The elastic properties, which are assumed to be isotropic, are the same for both phases (Young’s modulus E = 100 GPa and Poisson ratio ν = 0.45). The reference strain rate is set to

˙

ε0 = 1 s−1 for both phases and the strain rate sensitivity parameter m is either

equal to 1 (linear case) or 0.2 (non-linear case). In the AFF, SC-TF-SEC and MT-TF-AFF formulations, fibres are modeled with axisymmetric ellipsoidal inclusions elongated in the x3 direction and with an aspect ratio

of 1/100. The applied strain rate ˙E is isochoric and corresponds to in-plane
shear loading at 45◦ _{with respect to axis x}

1: ˙ E = ˙E11 1 0 0 0 −1 0 0 0 0 with ˙E11= 0.5 s−1 (75)

The calculated overall stress-strain responses obtained from the present SC-TF-AFF approach are first compared to the results given by the FFT method (Lahellec and Suquet, 2007b), the SEC (EIV+HS) approach (Lahellec and

0 0.01 0.02 0.03 0.04 0.05 0.06 0.07 0.08 0.09 0.1
0
50
100
150
200
250
300
350
400
450
500
E_{11}
Σ 11
(MPa)
FFT (Lahellec−Suquet, 2007)
SEC (EIV+HS) (Lahellec−Suquet, 2007)
MT-TF-AFF (Berbenni−Capolungo,2014)

SC-TF-SEC (Paquin et al., 1999) and SC-TF-AFF (present)

Figure 1. Overall (i.e. effective) monotonic responses obtained from different meth-ods for two-phase elasto-viscoplastic fibre-reinforced composites subjected to in– plane shear loading perpendicular to the fibres (fibre volume fraction f = 0.21, strain rate sensitivity parameter m = 1).

Suquet, 2007b) and the MT-TF-AFF approach (Berbenni and Capolungo, 2014) in figures 1 and 2 for two different strain-rate sensitivities m = 1 and m = 0.2, as initially done in Lahellec and Suquet (2007b).

Figure 1 reports the results of the SC-TF-AFF approach for m = 1 (linear case). In this case, both previous (Paquin et al., 1999) and present translated field approaches are equivalent and lead to the same results. The SC-TF (SEC or AFF) approach gives an overall response that is slightly stiffer than the ones obtained from the FFT method, the SEC (EIV+HS) approach or the MT-TF-AFF approach. In this case, this is clearly due to the self-consistent approximation itself applied to this two-phase microstructure with hard fibres being embedded in a soft matrix phase, for which the HS or the MT estimates classically represent a lower bound of the effective behavior for single-potential materials.

For m = 0.2 (non-linear case, see figure 2), more discrepancies occur between the different approximations and the FFT method especially at large physical times when the overall behavior tends to the viscoplastic asymptotic state. In this case, all the mean field approximations overestimate the FFT results. In comparison with the linear case, it is still observed that the asymptotic estimate given by the SC-TF-AFF approach is stiffer than the MT-TF-AFF one. However, in agreement with the FFT results, the transient regime de-termined with the present SC-TF-AFF approach is shorter than for m = 1. Furthermore, the present SC-TF-AFF approach provides results which are closer to the FFT response than the ones given by the original SC-TF-SEC

0 0.01 0.02 0.03 0.04 0.05 0.06 0.07 0.08 0.09 0.1 0 100 200 300 400 500 600 700 800 E 11 Σ 11 (MPa) FFT (Lahellec−Suquet, 2007) SEC (EIV+HS) (Lahellec−Suquet, 2007) MT-TF-AFF (Berbenni−Capolungo,2014) SC-TF-SEC (Paquin et al., 1999) SC-TF-AFF (present)

Figure 2. Overall (i.e. effective) monotonic responses obtained from different meth-ods for two-phase elasto-viscoplastic fibre-reinforced composites subjected to in– plane shear loading perpendicular to the fibres (fibre volume fraction f = 0.21, strain rate sensitivity parameter m = 0.2).

method. Also, for such microstructures with a relatively low volume fraction of fibres, these results (figures 1 and 2) confirm that the Mori-Tanaka’s es-timate, derived by Berbenni and Capolungo (2014), or the Hashin’s CCA, developed by Lahellec and Suquet (2007b), give more accurate results than the self-consistent scheme, especially regarding the asymptotic state at large physical times. However, for m = 0.2, figure 2 shows that the overall response calculated from the SC-TF-AFF approach during the transition from the elas-tic regime to the viscoplaselas-tic regime, i.e. up to E11=0.03, is close to the FFT

solution.

In figure 3, the phase average stress-strain responses (fibres with dotted lines, matrix with dashed lines) are reported in addition to the overall responses (solid lines) according to both the SC-TF-AFF and SC-TF-SEC approaches. It is observed that the overall stiffness and the average stress (i.e. the first mo-ment of stresses) in the fibres are largely overestimated with the SC-TF-SEC method of Paquin et al. (1999) while they are much reduced with the present SC-TF-AFF formulation. Thus, in comparison with the secant formulation originally developed by Paquin et al. (1999), the description of the mechanical behavior of two-phase materials is significantly improved with the proposed affine formulation.

Figure 3. Overall and phase average monotonic responses obtained from the present SC-TF-AFF affine approach and compared to the SC-TF-SEC secant approach (Paquin et al., 1999) for two-phase elasto-viscoplastic fibre-reinforced composites subjected to in-plane shear loading perpendicular to the fibres (fibre volume fraction f = 0.21, strain rate sensitivity parameter m = 0.2).

3.2 Polycristalline materials

In the case of polycrystalline materials, the local behavior of each crystal strongly depends on its orientation because of the anisotropy of plastic, elastic and thermal properties. As a result, the macroscopic behavior is importantly impacted by the internal stresses generated during a loading path because of the interactions between the different grains. In this section, different models are compared for various thermomechanical loading conditions: the proposed affine consistent model (labeled as SC-TF-AFF), the original secant self-consistent model of Paquin et al. (1999) (labeled as SC-TF-SEC) and the FFT-based spectral method (Lebensohn et al., 2012; Mareau et al., 2013; Moulinec and Suquet, 1998) (labeled as FFT). In the present case, the FFT-based spectral method uses the basic algorithm proposed by Moulinec and Suquet (1998) to solve the integral equation associated with the heterogeneous problem. In order to assess the validity of the proposed model, the results of the spectral method are taken as reference since this method provides a numerical solution to the integral equation without neglecting non-local interactions.

The polycrystal, which is used for the comparison, consists of 200 randomly oriented grains with spherical shape. In the case of the FFT-based spectral method, a 3D microstructure was generated using the procedure proposed by Robert et al. (2012). The different grains were initially approximated by spheroids being randomly positioned but not superimposed. The Watershed

algorithm (Meyer, 1994) was then used to dilate the spheroids to fill the volume element such that smooth grain boundaries were obtained. The microstructure was then discretized into a 128 × 128 × 128 regular grid.

3.2.1 Single crystal constitutive law

For the present comparison, the local behavior is described within a crystal plasticity framework. The phenomenological constitutive equations developed by M´eric and Cailletaud (1991) are used to model the behavior of each crys-tal. Considering a crystal with N slip systems, the constitutive law can be summarized in the following set of relations:

˙εth= α ˙T (76)
˙εvp=
N
X
s=1
1
2(m
s_{⊗ b}s_{+ b}s_{⊗ m}s_{) ˙γ}s _{(77)}
˙γs= h|τ
s_{− x}s_{| − r}s_{i}
Ks
!ns
sign (τs− xs) (78)
τs= σ : (bs⊗ ms) (79)
xs= asys with ˙ys= ˙γs− dsys| ˙γs| (80)
rs= rs_{0}+
N
X
t=1
QHstqt with ˙qt =1 − Bqt| ˙γt| (81)
In the above equations, ms _{and b}s _{are respectively the slip plane normal and}

the slip direction for the sth _{slip system. For each slip system, the viscoplastic}

shear strain rate ˙γs _{depends on:}

• the resolved shear stress τs _{which is connected to the stress tensor σ,}

• the isotropic hardening shear stress rs _{which is the force associated to the}

internal variable qs_{,}

• the kinematic hardening shear stress xs _{which is the force associated to the}

internal variable ys_{.}

Different material parameters have been introduced in the constitutive model: α is the thermal expansion tensor, K and n are viscosity parameters, a and d are kinematic hardening parameters and Q, B and H are isotropic hardening parameters. H is a N × N matrix providing a description of the interactions between the different slip systems.

3.2.2 Uniaxial tension

First, the case of a polycrystal subjected to uniaxial tension is considered. A constant macroscopic strain rate ( ˙E11 = 1 s−1) is imposed in the x1 direction

E (GPa) ν K (MPa) n

200 1/3 200 1, 5 and 10

Table 1

Material parameters for uniaxial tension simulations. Only non-zero coefficients are indicated. Single crystal elastic properties are assumed to be isotropic (E is the Young modulus and ν is the Poisson ratio).

while, except from Σ11, the macroscopic stress tensor components are set to

zero. The plastic flow rule is established for a f.c.c. crystal with slip systems belonging to the {111} < 110 > family. As shown in table 1, different set of parameters have been used. The set of parameters only differ by the value of the n exponent which varies from 1 to 10. These different n values allow testing the efficiency of the linearization procedure of the viscoplastic flow rule as a function of non-linearity.

The macroscopic stress-strain curves obtained with the different models and different set of parameters are plotted in figure 4. In the case of linear vis-coelasticity (i.e. n = 1), no difference is observed between the secant and affine formulations since they both yield the same exact definition of the viscoplastic compliances tensor. Also, the results obtained from the self-consistent models are very similar to the reference solution calculated with the spectral method in both the transient and asymptotic regimes. The good description of the transient regime indicates that the self-consistent approximation of the inte-gral equation provides a realistic representation of the interactions associated with the elasto-viscoplastic space-time couplings.

With an increasing non-linearity, both self-consistent models tend to overesti-mate the polycrystalline aggregate stiffness. However, no matter the value of n, the previsions of the proposed affine formulation are always closer to the reference solution. For the specific case of n = 5, the results can be compared to those obtained from the hereditary approach of Masson and Zaoui (1999) (labeled as SC-HER-AFF). This approach, which is based on the correspon-dence principle and an affine linearization procedure of the viscoplastic flow rule, requires a complex numerical implementation. Indeed, the solution is ob-tained from Laplace-Carson transforms whose inversion to the real time space is generally not trivial. Therefore, the proposed model is an interesting alter-native solution since it provides very similar results to the hereditary approach of Masson and Zaoui (1999) while the implementation is much easier.

Also, the previsions from the models are very different when the local stress and strain fields are examined. Figure 5 represents the situation of each grain in an equivalent stress-equivalent strain diagram at the end of the tension loading (E11 = 0.02) with the different models. It is observed that the dispersion of

the stress and strain fields is largely underestimated by both self-consistent models. For high n values, according to the secant formulation, the local strain

0 50 100 150 200 250 300 0 0.005 0.01 0.015 0.02

True stress (MPa)

True strain SC-TF-AFF SC-TF-SEC FFT 0 100 200 300 400 500 600 0 0.005 0.01 0.015 0.02

True stress (MPa)

True strain SC-TF-AFF SC-TF-SEC FFT SC-HER-AFF 0 100 200 300 400 500 600 0 0.005 0.01 0.015 0.02

True stress (MPa)

True strain

SC-TF-AFF SC-TF-SEC FFT

Figure 4. Macroscopic stress-strain curves calculated with the different models for a uniaxial tension test for different n values: n = 1 (top), n = 5 (middle) and n = 10 (bottom).

c1111 (GPa) c1122 (GPa) c1212 (GPa) K (MPa) n

197 125 122 12 11

r0 (MPa) Q (MPa) B a(MPa) d

40 10 3 40 000 1500

h1 h2 h3 h4 h5 h6

1 1 0.6 12.3 1.6 1.8

Table 2

Material parameters for cyclic plasticity simulations (316L stainless steel) (Guil-hem et al., 2013). Only independent elastic constants and non-zero coefficients are indicated.

field is almost equal to the prescribed macroscopic strain. Thus, the secant formulation provides results which are close to the upper bound estimation (i.e. ε (x, t) = E (t)) which is obtained from Taylor’s model (Taylor, 1938). On the contrary, the affine formulation yields a more realistic distribution of the stress and strain fields though important discrepancies with respect to the reference solution exist. The reason for these differences lies in the description of the influence of neighboring grains. While the spectral method explicitly accounts for neighboring effects as in a N-site modeling (Lebensohn, 2001), the present adopted 1-site self-consistent method describes the interactions between the different grains in an average manner through the properties of the reference homogeneous media. Consequently, on the contrary to the spectral method, self-consistent models do not account for the specific position of each grain.

3.2.3 Cyclic plasticity

The case of a 316L stainless steel polycrystalline aggregate subjected to a cyclic loading is now examined. The simulations are performed under strain control with various strain amplitudes (0.2 %, 0.4% and 0.8%) and with a constant loading frequency (1 Hz). The material properties, which are given in table 2, have been identified for 316L by Guilhem et al. (2013). Because of the f.c.c. crystal structure, only the {111} < 110 > plastic deformation mode is considered. The interaction matrix H is defined from six different terms (h1 to h6). They correspond to different types of interactions between a

given slip system and the other systems. Considering two slip systems (s and
t), the interaction term Hst _{depends whether the two considered systems are}

identical (Hst_{= h}

1), coplanar (Hst= h2), collinear (Hst= h3), Hirth junction

(Hst _{= h}

4), forming glissile junction (Hst = h5) or forming sessile junction

(Hst_{= h}
6).

mod-150 200 250 300 350 400 450 0.014 0.016 0.018 0.02 0.022 0.024 0.026 0.028

Equivalent stress (MPa)

Equivalent strain SC-TF-AFF SC-TF-SEC FFT 350 400 450 500 550 600 650 700 0.012 0.014 0.016 0.018 0.02 0.022 0.024 0.026 0.028 0.03

Equivalent stress (MPa)

Equivalent strain SC-TF-AFF SC-TF-SEC FFT 400 450 500 550 600 650 700 750 800 0.01 0.012 0.014 0.016 0.018 0.02 0.022 0.024 0.026 0.028 0.03

Equivalent stress (MPa)

Equivalent strain

SC-TF-AFF SC-TF-SEC FFT

Figure 5. Situation of each grain in an equivalent stress-equivalent strain diagram calculated with the different models at the end of the uniaxial tension simulations (E = 0.02) for different n values: n = 1 (top), n = 5 (middle) and n = 10 (bottom).

els, are plotted in figure 6 for the 10th_{loading cycle. When the strain amplitude}

is low (0.2%), a good agreement is observed between the spectral method and the self-consistent models. However, when the strain amplitude is increased (0.4% or 0.8%), kinematic hardening, which partly results from the develop-ment of internal stresses, is largely overestimated by the secant formulation. Indeed, as previously discussed, the secant formulation yields an overestima-tion of intergranular internal stresses such that kinematic hardening is poorly described with this model. On the contrary, the previsions of the cyclic stress-strain curves determined from the affine model and the spectral method are in very good agreement even for high strain amplitudes.

3.2.4 Creep

In order to test the ability of the different formulations to deal with the
cou-pling between thermoelasticity and viscoplasticity within the polycrystalline
material, creep simulations are performed. Creep simulations consist of two
steps: (i) temperature is first increased to 350◦_{C with a rate of 35} ◦_{C/s then}

(ii) a constant uniaxial stress (from 300 to 425 MPa) is applied to the
poly-crystalline aggregate for 105 _{s. The single crystal properties which are used}

for creep simulations were identified for a zirconium alloy (zircaloy-4, h.c.p.
crystal structure) at 350◦_{C by Diard et al. (2005). They are given in table}

3. Four different plastic deformation modes are considered in the simulations: prismatic slip {1010} < 1120 >, basal slip {0001} < 1120 >, pyramidal <a> slip {1011} < 1120 > and pyramidal <c+a> slip {1011} < 1123 >.

The strain rate, determined during the secondary creep stage, has been esti-mated using the different extensions (present affine and secant formulations) and compared to the results from the FFT-based spectral method. The results are reported in figure 7. For high stress values, the secant formulation under-estimates the stationary creep strain rate. This poor prevision of the creep behavior arises from the work hardening associated with the internal stresses which are known to be overestimated by the secant formulation. Thus, it is observed that the thermo-elasto-viscoplastic coupling is better described by the proposed affine formulation for which the agreement with the spectral method is good for any applied stress. This result indicates that the partial relaxation of internal stresses during the second loading step is well captured by the affine model.

Also, the slope of the strain rate versus stress curve corresponds to the tive strain rate sensitivity of the polycrystalline aggregate. While the effec-tive strain rate sensitivity varies smoothly according to the spectral method, abrupt changes are observed with both self-consistent models. These strain rate sensitivity variations can be explained from the activation of the different deformation modes. Indeed, in the case of zircaloy-4, four deformation modes

-200 -150 -100 -50 0 50 100 150 200 -0.002 -0.0015 -0.001 -0.0005 0 0.0005 0.001 0.0015 0.002

True stress (MPa)

True strain SC-TF-AFF SC-TF-SEC FFT -250 -200 -150 -100 -50 0 50 100 150 200 250 -0.004 -0.003 -0.002 -0.001 0 0.001 0.002 0.003 0.004

True stress (MPa)

True strain SC-TF-AFF SC-TF-SEC FFT -300 -200 -100 0 100 200 300 -0.008 -0.006 -0.004 -0.002 0 0.002 0.004 0.006 0.008

True stress (MPa)

True strain SC-TF-AFF

SC-TF-SEC FFT

Figure 6. Macroscopic stress-strain curves obtained for a 316L polycrystal subjected to strain-controlled cyclic loadings with different strain amplitudes: 0.2% (top), 0.4% (middle) and 0.8% (bottom). The results correspond to the 10th cycle.

c1111 (GPa) c3333 (GPa) c1122 (GPa) c2233 (GPa) c1212 (GPa)
103.2 118.3 51.6 46.6 23
α_{11} (K−1_{)} _{α}
33 (K−1)
5.3 × 10−6 _{1.01 × 10}−5
Prismatic

r0 (MPa) K (MPa) n a(MPa) d

20 198 9.4 22 100 170 Basal r0 (MPa) K (MPa) n 132 90 5.5 Pyramidal <a> r0 (MPa) K (MPa) n 107 500 7.5 Pyramidal <c+a>

r0 (MPa) K (MPa) n a(MPa) d

195 55 11.3 6 120 170

Table 3

Material parameters for creep simulations (zircaloy-4) (Diard et al., 2005). Only independent elastic constants and non-zero coefficients are indicated.

1e-09 1e-08 1e-07 1e-06

300 320 340 360 380 400 420

Stationary strain rate (1/s)

Stress (MPa) SC-AFF

SC-SEC FFT

Figure 7. Steady creep strain rate calculated with the different extensions (present affine and secant formulations) and the FFT method for a zircaloy-4 polycrystalline aggregate as a function of the applied stress.

with different strain rate sensitivities exist. As a result, the evolution of the effective strain rate sensitivity strongly depends on the active deformation modes. According to the FFT method, the activation of a deformation mode in a given grain occurs progressively when the applied stress is increased since intragranular fluctuations of the stress field are accounted for. On the contrary, self-consistent models consider only the volume average strain and stress ten-sors in each grain to determine the overall behavior. Thus, the activation of a deformation mode takes place simultaneously over the entire grain volume. The abrupt strain rate sensitivity variations being observed at a macroscopic scale with both self-consistent models are therefore caused by the rapid tran-sitions from one deformation mode to another occurring in different grains.

4 Conclusions

Translated field techniques were used to build up a new self-consistent model for materials with a local thermo-elasto-viscoplastic behavior. The present homogenization scheme is based on a first order affine linearization of the vis-coplastic flow rule inspired from the initial work of Masson et al. (2000). The proposed model can be seen as an extension of the classical secant formula-tion first developed for elasto-viscoplastic materials by Paquin et al. (1999) without altering the CPU time needed for computations. When compared to reference solutions calculated from a FFT spectral method, a good description of the thermomechanical behavior is obtained with the present model. More specifically, in comparison with the original secant formulation, the descrip-tion of the interacdescrip-tions between the different phases of a representative volume element is largely improved with the proposed affine model. Furthermore, al-though the spatial inter-granular elasto-viscoplastic interactions are complex, the present model does not require intensive computations since it is entirely formulated in the real-time space. It is an alternative approach to other recent polycristalline models (e.g. Wang et al., 2010) that should be considered with interest for applications where the computation time is a critical issue, e.g. fatigue, creep responses of polycrystalline materials.

Acknowledgments

One of the author (S.B.) would like to thank the support of the French State through the National Research Agency (ANR) under the program Investment in the future (Labex DAMAS referenced as ANR-11-LABX-0008-01).

References

Berbenni, S., Capolungo, L., 2014. A Mori-Tanaka homogenization scheme for non-linear elasto-viscoplastic heterogeneous materials based on translated fields: an affine extension. Comptes Rendus de Mecanique (special issue), accepted for publication.

Berbenni, S., Favier, V., Lemoine, X., Berveiller, M., 2004. Micromechanical modeling of the elastic-viscoplastic behavior of polycrystalline steels having different microstructures. Materials Science Engineering A 372, 128-136. Brassard, L., Stainier, L., Doghri, I., Delannay, L., 2012. Homogenization of

elasto-(visco)plastic composites based on an incremental variational princi-ple. International Journal of Plasticity 36, 86-112.

Diard, O., Leclercq, S., Rousselier, G., Cailletaud, G., 2005. Evaluation of finite element based analysis of 3D multicrystalline aggregates plasticity: Application to crystal plasticity model identification and the study of stress and strain fields near grain boundaries. International Journal of Plasticity 21, 691-722.

Gilormini, P., 1995. Insuffisance de l’extension classique du mod`ele auto-coh´erent au comportement non lin´eaire. Comptes Rendus Academie des Sciences Paris 320, 115-122.

Guilhem, Y., Basseville S., Curtit, F., St´ephan, J.M., Cailletaud, G., 2013. Numerical investigations of the free surface effect in three-dimensional poly-crystalline aggregates. Computational Materials Science 70, 150-162. Harren, S.V., 1991. The finite deformation of rate dependent polycrystals I

and II. Journal of the Mechanics and Physics of Solids 39, 345-383.

Hashin, Z., 1969. The inelastic inclusion problem. International Journal of Engineering Science 7, 11-36.

Hershey, A.V., 1954. The elasticity of an isotropic aggregate of anisotropic cubic crystals. ASME, Journal of Applied Mechanics 21, 236-240.

Hill, R., 1965. Continuum micro-mechanics of elastoplastic polycrystals. Jour-nal of the Mechanics and Physics of Solids 13, 89-101.

Hutchinson, J.W., 1976. Bounds and self-consistent estimates for creep of poly-crystalline materials. Proceedings of the Royal Society of London A 348, 101-127.

Kr¨oner, E., 1958. Berechnung der elastischen Konstanten des Vielkristalls aus den konstanten des Einskristalls. Zeitschrift fur Physik 151, 504.

Kr¨oner, E., 1961. Zur plastischen Verformung des Vielkristalls. Acta Metal-lurgica 9, 155-161.

Kr¨oner, E., 1989. Modified green functions in the theory of heterogeneous and/or anisotropic linearly elastic media, in: Weng, G.J., Taya, M., Abe, M. (Eds.), Micromechanics and inhomogeneity, Springer, Berlin, pp. 197-211.

Lahellec, N., Suquet, P., 2007. Effective behavior of linear viscoelastic com-posites: A time-integration approach. International Journal of Solids and Structures 44, 507-529.

Lahellec, N., Suquet, P., 2007. On the effective behavior of nonlinear inelastic composites: I. Incremental variational principles. Journal of the Mechanics and Physics of Solids 55, 1932-1963.

Lahellec, N., Suquet, P., 2013. Effective response and field statistics in elasto-plastic and elasto-viscoelasto-plastic composites under radial and non radial load-ings. International Journal of Plasticity 42, 1-30.

Laws, N., McLaughlin, R., 1978. Self-consistent estimates for the viscoelastic creep compliances of composite materials. Proceedings of the Royal Society of London A 359, 251-273.

Lebensohn, R.A., Tom´e, C.N., 1993. A self-consistent anisotropic approach for the simulation of plastic deformation and texture development of polycrys-tals: Application to zirconium alloys. Acta Metallurgica et Materialia 41, 2611-2624.

Lebensohn, R.A., 2001. N-site modeling of a 3D viscoplastic polycrystal using Fast Fourier Transform. Acta Materialia 49, 2723-2737.

Lebensohn, R.A., Kanjarla, A.K., Eisenlohr, P., 2012. An elasto-viscoplastic formulation based on fast fourier transforms for the prediction of microme-chanical fields in polycrystalline materials. International Journal of Plastic-ity 32-33, 59-69.

Levin, V.M., 1967. Thermal expansion coefficients of heterogeneous materials. Mekhanika Tverdogo Tela 2, 8894 (English translation: Mechanics of Solids 11, 5861).

Mareau, C., Cuillerer, D., Morel, F., 2013. Experimental and numerical study of the evolution of stored and dissipated energies in a medium carbon steel under cyclic loading. Mechanics of Materials 60, 93-106.

Masson, R., Zaoui, A., 1999. Self-consistent estimates for the rate-dependent elastoplastic behaviour of polycrystalline materials. Journal of the Mechan-ics and PhysMechan-ics of Solids 47, 1543-1568.

Masson, R., Bornert, M., Suquet, P., Zaoui, A., 2000. Affine formulation for the prediction of the effective properties of nonlinear composites and poly-crystals. Journal of the Mechanics and Physics of Solids 48, 1203-1227. Mercier, S., Molinari, A., 2009. Homogenization of elasticviscoplastic

hetero-geneous materials: Self-consistent and Mori-Tanaka schemes. International Journal of Plasticity 25, 1024-1048.

Mercier, S., Molinari, A., Berbenni, S., Berveiller, M., 2012. Comparison of different homogenization approaches for elastic-viscoplastic materials. Mod-elling and Simulation in Materials Science and Engineering 20, 024004. M´eric, L., Cailletaud, G., 1991. Single crystal modeling for structural

calcula-tions: Part 2 - Finite element implementation. ASME, Journal of Engineer-ing Materials and Technology 113, 171-182.

Meyer, F., 1994. Topographic distance and watershed lines. Signal Processing 38, 113-125.

Molinari, A., Canova, G.R., Ahzi, S., 1987. A self consistent approach of the large deformation polycrystal viscoplasticity. Acta Metallurgica 35, 2983-2994.

Molinari, A., Ahzi, S., Kouddane, R., 1997. On the self-consistent modeling of elasticplastic behavior of polycrystals. Mechanics of Materials 26, 43-62. Molinari, A., 2002. Averaging models for heterogeneous viscoplastic and elastic-viscoplastic materials.Trans. ASME, Journal of Engineering Mate-rials and Technology 124, 62-70.

Moulinec, H., Suquet, P., 1998. A numerical method for computing the overall response of nonlinear composites with complex microstructure. Computer Methods in Applied Mechanics and Engineering 157, 69-94.

Mura, T., 1987. Micromechanics of defects in solids. Kluwer Academic Pub-lishers, Dordrecht, The Netherlands.

Nemat-Nasser, S., Obata, M., 1986. Rate-dependent, finite elasto-plastic de-formation of polycrystals. Proceedings of The Royal Society of London A 407, 343-375.

Nemat-Nasser, S., Hori, M., 1994. Micromechanics: Overall Properties of Het-erogeneous Materials, North-Holland Series in Applied Mathematics and Mechanics.

Paquin, A., Sabar, H., Berveiller, M., 1999. Integral formulation and self-consistent modelling of elastoviscoplastic behavior of heterogeneous mate-rials. Archive of Applied Mechanics 69, 14-35.

Pierard, O., Doghri, I., 2006. An enhanced affine formulation and the corre-sponding numerical algorithms for the mean-field homogenization of elasto-viscoplastic composites. International Journal of Plasticity 69, 131-157. Pierard, O., Llorca, J., Segurado, J., Doghri, I., 2007. Micromechanics of

particle-reinforced elasto-viscoplastic composites: Finite element versus affine homogenization. International Journal of Plasticity 23, 1041-1060. Rekik, A., Auslender, F., Bornert, M., Zaoui, A., 2007. Objective evaluation

of linearization procedures in non linear homogenization: a methodology and some implications on the accuracy of micromechanical schemes. Inter-national Journal of Solids and Structures 44, 3468-3496.

Robert, C., Saintier, N., Palin-Luc, T., Morel, F., 2012. Micro-mechanical modelling of high cycle fatigue behaviour of metals under multiaxial loads. Mechanics of Materials 55, 112-129.

Rougier, Y., Stolz, C., Zaoui, A., 1994. Self-consistent modelling of elasticvis-coplastic polycrystals. Comptes Rendus Academie des Sciences Paris 318, 145-51.

Sabar, H., Berveiller, M., Favier, V., Berbenni, S., 2002. A new class of micro-macro models for elasticviscoplastic heterogeneous materials. International Journal of Solids and Structures 39, 3257-3276.

Taylor, G.I., 1938. Plastic strain in metals. Journal Institute of Metals 61, 307-324.

Wang, H., Wu, P.D., Tom´e, C.N., Huang, Y., 2010. A finite strain elastic-viscoplastic self-consistent model for polycrystalline materials. Journal of the Mechanics and Physics of Solids 58, 594-612.

Weng, G.J., 1981. Self-consistent determination of time-dependent behavior of metals. ASME, Journal of Applied Mechanics 48, 41-46.

Weng, G.J., 1981. A self-consistent scheme for the relaxation behaviour of metals. ASME, Journal of Applied Mechanics 48, 779-784.

Zaoui, A., Raphanel, J.L., 1993. On the nature of the intergranular accom-modation in the modeling of elastoviscoplastic behavior of polycrystalline aggregates, in: Teodosiu, C. et al (Eds.), Mecamat 91: Large Plastic Defor-mations, Fundamentals and Application to Metal Forming, Rotterdam, pp. 185-92.